Ester-Based Electrolytes for Low- Temperature Li-Ion Cells
NASA's Jet Propulsion Laboratory, Pasadena, California
Electrolytes comprising LiPF6 dissolved at a concentration of 1.0 M in five different solvent mixtures of alkyl carbonates have been found to afford improved performance in rechargeable lithium-ion electrochemical cells at temperatures as low as -70° C. These and other electrolytes have been investigated in continuing research directed toward extending the lower limit of practical operating temperatures of Li-ion cells. This research at earlier stages, and the underlying physical and chemical principles, were reported in numerous previous NASA Tech Briefs articles, the most recent being "Low-ECContent Electrolytes for Low-Temperature Li-Ion Cells" (NPO-30226), NASA Tech Briefs, Vol. 27, No. 1 (January 2003), page 46. The ingredients of the present solvent mixtures are ethylene carbonate (EC), ethyl methyl carbonate (EMC), methyl butyrate (MB), methyl propionate (MP), ethyl propionate (EP), ethyl butyrate (EB), and ethyl valerate (EV). In terms of volume proportions of these ingredients, the present solvent mixtures are
1EC + 1EMC + 8MB,
1EC + 1EMC + 8EB,
1EC + 1EMC + 8MP,
1EC + 1EMC + 8EV, and
1EC + 9EMC.
These electrolytes were placed in Li-ion cells containing carbon anodes and LiNi0.8Co0.2O2 cathodes, and the low-temperature electrical performances of the cells were measured. The cells containing the MB and MP mixtures performed best.
This work was done by Marshall Smart and Ratnakumar Bugga of Caltech for NASA's Jet Propulsion Laboratory. For further information, access the Technical Support Package (TSP) free on-line at www.techbriefs.com/tsp under the Physical Sciences category. NPO-41097
This Brief includes a Technical Support Package (TSP).
Ester-Based Electrolytes for Low-Temperature Li-Ion Cells
(reference NPO-41097) is currently available for download from the TSP library.